Crystal design by CH···N and N···N interactions: high-pressure structures of high-nitrogen-content azido-triazolopyridazines compounds
Olejniczak, Anna; Katrusiak, Anna; Podsiadło, Marcin; Katrusiak, Andrzej; Acta Crystallographica Section B 76 (2020) –; doi:10.1107/S2052520620014493

data_2108708
_publ_section_title
;
 Crystal design by CH&#x00B7;&#x00B7;&#x00B7;N and
 N&#x00B7;&#x00B7;&#x00B7;N interactions: high-pressure structures of
 high-nitrogen-content azido-triazolopyridazines compounds
;
_journal_coeditor_code           DK5103SUP1
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first
;
;
_journal_paper_doi               10.1107/S2052520620014493
_journal_volume                  76
_journal_year                    2020
_chemical_formula_moiety         'C5 H3 N7'
_chemical_formula_sum            'C5 H3 N7'
_chemical_formula_weight         161.14
_chemical_name_systematic        6-azido-1,2,4-triazolo[4,3-b]pyridazine
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_audit_creation_date             2018-10-29
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_cell_angle_alpha                90
_cell_angle_beta                 94.6(2)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.918(15)
_cell_length_b                   18.223(2)
_cell_length_c                   8.897(14)
_cell_measurement_pressure       770000
_cell_measurement_reflns_used    890
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      21.3310
_cell_measurement_theta_min      4.0520
_cell_volume                     1280(3)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.31 (release 14-01-2014 CrysAlis171 .NET)
(compiled Jan 14 2014,18:38:05)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.31 (release 14-01-2014 CrysAlis171 .NET)
(compiled Jan 14 2014,18:38:05)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.31 (release 14-01-2014 CrysAlis171 .NET)
(compiled Jan 14 2014,18:38:05)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_environment      'diamond-anvil cell'
_diffrn_ambient_pressure         770000
_diffrn_ambient_temperature      296(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.2413
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 0.179
_diffrn_measured_fraction_theta_max 0.158
_diffrn_measurement_details
;
  1 phi    -35.00   19.75   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
   0.0000  -30.0000    0.0000     -     73

  2 phi    140.00  200.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
   0.0000  -30.0000    0.0000     -     80

  3 phi    160.00  217.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
   0.0000   30.0000    0.0000     -     76

  4 phi    -20.00   34.75   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
   0.0000   30.0000    0.0000     -     73

  5 omega  -24.00   24.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -       30.0000   39.4600  -12.9000 64

  6 omega  -24.00   24.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -       30.0000   39.4600  167.1000 64

  7 omega  -50.00   10.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -      -30.0000   39.4600  167.1000 80

  8 omega  -50.00   10.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -      -30.0000   39.4600  -12.9000 80

  9 omega  -64.00   -8.50   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -      -30.0000   81.4000  -28.9000 74

 10 omega  -64.00   -8.50   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -      -30.0000   81.4000  151.1000 74

 11 omega  -19.00    8.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -       30.0000   81.4000  151.1000 36

 12 omega  -19.00    8.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -       30.0000   81.4000  -28.9000 36

 13 omega  -43.00  -21.25   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -       30.0000  134.6000  -56.9000 29

 14 omega  -43.00  -21.25   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -       30.0000  134.6000  123.1000 29

 15 omega  -90.00  -36.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -      -30.0000  134.6000  123.1000 72

 16 omega  -90.00  -36.00   0.7500   37.0000
omega____ theta____ kappa____ phi______ frames
    -      -30.0000  134.6000  -56.9000 72
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'KM-4 CCD'
_diffrn_measurement_method
;
HP omega scans - for more details see:
A. Budzianowski, A. Katrusiak in High-Pressure Crystallography
(Eds.: A. Katrusiak, P. F. McMillan),
Dordrecht: Kluwer Acad. Publ., 2004 pp.157-168
;
_diffrn_orient_matrix_UB_11      0.0623906000
_diffrn_orient_matrix_UB_12      0.0004926000
_diffrn_orient_matrix_UB_13      -0.0527266000
_diffrn_orient_matrix_UB_21      0.0321401000
_diffrn_orient_matrix_UB_22      0.0336272000
_diffrn_orient_matrix_UB_23      0.0307576000
_diffrn_orient_matrix_UB_31      0.0561843000
_diffrn_orient_matrix_UB_32      -0.0196570000
_diffrn_orient_matrix_UB_33      0.0515619000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1603
_diffrn_reflns_av_unetI/netI     0.0584
_diffrn_reflns_Laue_measured_fraction_full 0.179
_diffrn_reflns_Laue_measured_fraction_max 0.158
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            4666
_diffrn_reflns_point_group_measured_fraction_full 0.179
_diffrn_reflns_point_group_measured_fraction_max 0.158
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.928
_diffrn_reflns_theta_min         4.066
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    0.123
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.73408
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.31 (release 14-01-2014 CrysAlis171 .NET)
(compiled Jan 14 2014,18:38:05)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.673
_exptl_crystal_description       plate
_exptl_crystal_F_000             656
_exptl_crystal_size_max          0.36
_exptl_crystal_size_mid          0.29
_exptl_crystal_size_min          0.18
_refine_diff_density_max         0.131
_refine_diff_density_min         -0.136
_refine_diff_density_rms         0.039
_refine_ls_extinction_coef       0.015(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.077
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     98
_refine_ls_number_reflns         438
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.077
_refine_ls_R_factor_all          0.1114
_refine_ls_R_factor_gt           0.0714
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1550P)^2^+0.2012P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1981
_refine_ls_wR_factor_ref         0.2310
_reflns_Friedel_coverage         0.000
_reflns_number_gt                267
_reflns_number_total             438
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            dk5103sup1.cif
_cod_data_source_block           C5H3N7at0.77GPa
_cod_database_code               2108708
_cod_database_fobs_code          2108708
_shelx_shelxl_version_number     2014/7
_reflns_odcompleteness_completeness 15.91
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.87
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
2.a Aromatic/amide H refined with riding coordinates:
 C27(H27), C28(H28), C23(H23), C7(H7), C8(H8), C3(H3)
;
_olex2_submission_special_instructions 'No special instructions were received'